show - HZG
of the original manuscript:
Boesenberg, U.; Pistidda, C.; Tolkiehn, M.; Busch, N.; Saldan, I.;
Suarez-Alcantara, K.; Arendarska, A.; Klassen, T.; Dornheim, M.:
Characterization of metal hydrides by in-situ XRD
In: International Journal of Hydrogen Energy (2014) Elsevier
Characterization of metal hydrides by in-situ XRD
Ulrike Bösenberga, Claudio Pistiddaa, Martin Tolkiehnb, Nina Buscha, Ivan Saldana,
Karina Suarez-Alcantaraa, Anna Arendarskaa, Thomas Klassena, Martin Dornheima,*
Institute of Materials Research, Helmholtz-Zentrum Geesthacht, Max-Planck-Straße 1, D-
21502 Geesthacht , Germany.
HASYLAB, Deutsches-Elektronen-Synchrotron DESY, Notkestraße 85, D-22607 Hamburg,
*Corresponding author. Tel.: +49 4152 87 2604; fax: +49 4152 87 2625. E-mail address:
[email protected] (M. Dornheim).
In-situ synchrotron radiation powder X-ray diffraction (SR-PXD) technique is a powerful tool
to gain a deeper understanding of reaction mechanisms in crystalline materials. In this paper,
the implementation of a new in-situ SR-PXD cell for solid-gas reactions is described in detail.
The cell allows performing measurements in a range of pressure which goes from light
vacuum (10-2 bar) up to 200 bar and temperatures from room temperature up to 550°C. The
high precision, with which pressure and temperature are measured, enables to estimate the
thermodynamic properties of the observed changes in the crystal structure and phase
Keywords: In-situ XRD, metal hydrides, complex hydrides, hydrogen storage
The understanding of the solid-gas reactions kinetics and their dependence on the
applied conditions (i.e. gas pressure and temperature) are key requirements to design
novel materials for hydrogen storage purposes. In this regards, in-situ SR-PXD has been
proven to be a very powerful tool to gain information on material properties and reaction
kinetics. [1-5] X-ray scattering generally requires short data acquisition times and shows high
penetration depths, especially for low Z materials, therefore, it is a very suitable technique for
in-situ studies of chemical reactions. While upon hydrogenation and de-hydrogenation the
interstitial hydrides typically show considerable changes in the unit cell volume , complex
hydrides and Reactive Hydride Composites (RHC) show nucleation and growth of new
phases with completely different crystal structures and atom arrangements . The formation
and stability of these new phases depend on the applied pressure and temperature conditions.
The temperature/pressure equilibrium conditions are function of the enthalpy and entropy of
the reaction, in simple cases, such as MgH2, this is determined by the enthalpy of the MgH2
formation (-75 kJ/molH2)  and the hydrogen entropy change (130 J/Kmol) .
In the last decades, owing to their favourable thermodynamic properties and high hydrogen
capacities, the so called Reactive Hydride Composites (RHC) have been considered as
possible candidates for hydrogen storage systems for mobile applications . However, the
hydrogen absorption and desorption reactions of these systems are rather complex. For the
LiBH4-MgH2 system, in-situ SR-PXD significantly contributed to the understanding of the
reaction pathway [1, 2]. In contrast, the exact reaction pathway for the Ca(BH4)2-MgH2
system or even Ca(BH4)2 alone, is still unclear because of the number of intermediate phases
and side reactions involved in the hydrogen desorption and absorption processes [9-12].
Yartys et al.  have demonstrated how the possibility to perform in-situ neutron diffraction
analysis, acquiring simultaneously thermodynamic properties, is important for the
characterization of high-pressure interstitial hydrides.
In this work, a newly-designed sample cell for in situ SR-PXD analysis and its experimental
setup at Beamline D3, HASYLAB, DESY are described in detail. Owing to its fast reaction
kinetics in a suitable temperature and pressure range, MgH2 doped with Nb2O5 was selected
for testing the setup [14-17]. The experiments carried out at several hydrogen pressures on the
doped MgH2 show, as expected, a clear dependence of the sorption temperature on the applied
pressure. Quantitative analysis of the diffracted intensity relates the chemical reaction to
pressure and temperature. In addition, the in-situ cell was employed for investigating the
absorption reaction of the RHC system CaH2-MgB2 at hydrogen pressure of 120 bar and
temperature of 350°C.
Although, in this work the cell was used for the study of hydrogen storage materials, it can be
employed in the study of all sorts of solid-gas reactions. Due to the sensitive nature and high
reactivity of the material in powder form, the cell is designed in such a way, that it can be
mounted under inert atmosphere in a glove box.
The used sample cell is a modification of previously developed cells used for studies of
catalytic reactions using a flow of gas or liquids through a powder bed as well as studies of
solid-gas reactions in metal hydrides [5, 18, 19]. A schematic drawing of the sample cell is
shown in figure 1a. The implementation of the sample cell at the Beamline D3, HASYLAB,
DESY is shown in figure 1b.
The cell is attached using a standard goniometer head on a Huber 4-circle diffractometer. The
sample material, in this case powder, is inserted in a single crystal sapphire capillary with an
outer diameter of 1.1mm (Saint Gobain Crystals), matching standard 1/16” Swagelok nuts.
These sapphire capillaries can withstand temperatures up to 2000°C and pressures up to 900
bar , moreover, they are chemically inert and transparent to a high energy X-ray beam .
For our experiments the sample cell was introduced in an argon filled glove box to perform
the loading of the sample under inert conditions.
To insure tightness for pressures up to 200 bar hydrogen, vespel ferrules (15% Graphite 85%
Vespel® ferrules for Gas Chromatography from SGE) are used to tighten the Swagelok nuts
and mounting the capillary. The gas is equally distributed on the sample from both sides using
a 1/16” stainless steel tube between the two Swagelok nuts fixing the capillary. A type K
thermocouple inserted into the powder bed in the capillary measures and controls (via a
standard PID controller) the sample temperature during the experiment. The sample is heated
using a ceramic heating element from BACH GmbH. The heating element is placed on the
rails below the sample capillary and its position can be adjusted for each sample. For
mounting the capillary it can be conveniently lowered and moved along the rails. Its operation
is controlled by the thermocouple inserted in the powder bed via a PID control from JUMO
GmbH, Fulda, Germany. The temperature program is set by using the corresponding
software, where the temperature is recorded, also.
Pressures in the range from 10-2 to 200 bar can be applied using a stainless gas system
equipped with Swagelok manual valves. The pressure is monitored and recorded using a
WIKA pressure gauge (Alexander Wiegand GmbH) and the corresponding EasyCom
software supplied by the manufacturer.
The measurements were carried out at the D3 Beamline at HASYLAB, DESY, Hamburg. A
silicon (111) double crystal monochromator was used to select a wavelength of = 0.5003 Å.
Diffraction data were collected using a MarCCD 165 2-dimensional detector (Marresearch
GmbH). For normalization the intensity of the incident beam was measured using a NaJdetector looking at a scatter foil.
3. Results and discussion
To illustrate the power of this method and the sample cell, measurements with magnesium
hydride, catalyzed with 5 mol% Nb2O5 were measured under approximately 5, 10 and 15 bar
hydrogen; the exact values are noted with the experiments in figure 2. In each measurement,
the sample was heated up to 450°C with 5 K/min and after an isothermal period of 5 min
cooled down to room temperature, also with 5 K/min. The results are shown in figure 2, a, b
and c. Below the X-ray diffraction data the temperature, pressure and peak area for MgH2 and
Mg as a measure of quantity is plotted for each experiment. The pressure was measured in
relative units, that means that p = 0 bar is equivalent to atmospheric pressure.
The correlation between the change in pressure and the sorption reaction is striking. As the
temperature reaches the equilibrium temperature for the chosen pressure, e.g. 345°C for the
experiment performed under 5 bar hydrogen pressure, immediate desorption of MgH2 into
metallic Mg can be observed. This is followed by a distinct rise in pressure of about 0.15 bar.
Qualitative analysis clearly correlates the desorption reaction to a fast decrease in the
intensities of the MgH2 reflections and to a formation and increase in intensity of metallic Mg
reflections. During the cooling, the opposite effect is observed. As the pressure decreases
again, at a slightly lower temperature than the one of the previous desorption reaction, the
intensities of the Mg reflections decrease and vanish while the up-rise of the MgH2 reflections
can be observed. For the analysis of the relative changes in the phase fractions, peak areas of
the MgH2 (110) and Mg (102) reflections were evaluated. The lack of diffraction data in the
middle of the experiment at 10 bar hydrogen is due to refilling of the synchrotron storage
Increasing the applied hydrogen pressure a clear increment of desorption temperatures is
noted. Besides the changes in the material sorption properties, variations of the material phase
composition are visible. As the measurements start from nanocrystalline MgH2 with a mixture
of and phase, the -phase vanishes during the first heating and is not reformed during
cooling. The decrease of the full width at half maximum of the MgH2 intensities is caused by
coarsening of the MgH2 crystallites. It also occurs mainly during the first heating and
desorption reaction but continues upon cycling at these high temperatures. Furthermore, the
weak reflexes of Nb2O5 can be observed. The reflections remain weak with the ongoing
sorption processes, indicating that the material nanostructure remains constant. Furthermore
reaction between Nb2O5 with MgH2 or Mg can be observed, resulting in the final formation of
MgO, as previously reported by Friedrichs et al. .
The pressure changes in the in-situ cell caused by the heating/cooling of the sample are
negletable. In fact, the overall inner volume of the in-situ cell is roughly 2 mL, whereas, the
volume of the heated portion of the cell (i.e. the capillary) is only about 0.005 mL.
Furthermore, as the pressure is measured continuously throughout the experiment, the
pressure changes caused by the temperature changes can be subtracted as a linear baseline.
For future experiments the synchronisation of the recording system for diffraction frames,
temperature and pressure will be optimized to access highly precise information.
The application of higher pressures and the investigation of more complex systems are well
feasible. As an example, the first absorption reaction of the RHC system CaH2-MgB2 under
120 bar hydrogen and a temperature of 350°C is shown in figure 3.
As the initial CaH2-MgB2 material is heated, the CaH2 peaks intensity becomes more
pronounced, due to crystallite coarsening. In the isothermal period, clearly the formation of Ca(BH4)2 and MgH2 can be observed. The lack of diffraction data after 1.5 hours into the
experiment is due to injection at the synchrotron storage ring. The pressure is rather stable
over the whole experiment, starting at 121 bar hydrogen a value of 117 bar is reached at the
end of the experiment. The linear decrease by 4 bar is due to a small leakage. During the last
scans of the cooling a phase transformation from -Ca(BH4)2 to -Ca(BH4)2 can be observed.
The slow reaction kinetics in combination with the slight hydrogen-leakage do not allow
tracing the absorption reaction as a decrease in pressure.
In conclusion, in-situ SR-PXD is an extremely powerful tool to investigate solid-gas
reactions, e.g. hydrogen sorption reactions of metal hydrides. The ongoing reactions and
phase transformations can be characterized as a function of pressure and temperature.
Recording of pressure and temperature throughout the whole experiment allows for powerful
conclusions on the reaction pathway and even thermodynamic properties, especially in
combination with quantitative analysis. The newly implemented setup at Beamline D3,
HASYLAB, DESY allows measurements in environments up to 200 bar hydrogen and 550°C.
The authors thank Klaus Pranzas, Mathias Herrmann and Dennis Heims for experimental
support. The authors are especially grateful Dr. Torben R. Jensen, Aarhus University,
Denmark for his help and support. Financial support of the German Chinese Sustainable Fuel
Initiative is gratefully acknowledged. This work was supported by the European Community
under MRTN-Contract “Complex Solid State Reactions for Energy Efficient Hydrogen
Figure 1 a) Schematic drawing of the in-situ sample cell and b) its implementation at Beamline D3,
HASYLAB, DESY. The insert magnifies the sample within the capillary and the heater placed beneath.
Figure 2 In-situ XRD of MgH2 under different hydrogen pressures a) p = 5bar H2, b) 10bar H2 and
c) 15bar H2. Below the diffracted patterns quantitative analysis of the diffracted intensities of the MgH2
(110) peak and the Mg (102) are plotted. Furthermore, the absolute pressure as well as the sample cell
is plotted. All data are correlated to each other by measurement time.
Figure 3 In-situ XRD of an absorption reaction in CaH2-MgB2 composites measured at 120 bar
hydrogen, holding approx. 2.5 hours isothermal at 350°C.
 Bösenberg U, Doppiu S, Mosegaard L, Barkhordarian G, Eigen N, Borgschulte A, et al.
Hydrogen sorption properties of MgH2–LiBH4 composites. Acta Mater 2007;55:3951-8.
 Bösenberg U, Ravnsbæk DB, Hagemann H, D’Anna V, Minella CB, Pistidda C, et al.
Pressure and temperature influence on the desorption pathway of the LiBH4−MgH2 composite
system. J Phys Chem C 2010;114:15212-7.
 Gross KJ, Guthrie S, Takara S, Thomas G. In-situ X-ray diffraction study of the
decomposition of NaAlH4. J Alloy Compd 2000;297:270-81.
 Jensen TR, Andreasen A, Vegge T, Andreasen JW, Ståhl K, Pedersen AS, et al.
Dehydrogenation kinetics of pure and nickel-doped magnesium hydride investigated by in
situ time-resolved powder X-ray diffraction. Int J Hydrogen Energ 2006;31:2052-62.
 Jensen TR, Nielsen TK, Filinchuk Y, Jorgensen J-E, Cerenius Y, Gray EM, et al. Versatile
in situ powder X-ray diffraction cells for solid-gas investigations. J Appl Crystallogr
 Buchner H. Energiespeicherung in Metallhydriden. Wien: Springer; 1982.
 Lide DR. Handbook of Chemistry and Physics. Boca Raton: CRC Press; 1994.
 Dornheim M, Eigen N, Barkhordarian G, Klassen T, Bormann R. Tailoring hydrogen
storage materials towards application. Adv Eng Mater 2006;8:377-85.
 Barkhordarian G, Jensen TR, Doppiu S, Bosenberg U, Borgschulte A, Gremaud R, et al.
Formation of Ca(BH4)2 from hydrogenation of CaH2+MgB2 composite. J Phys Chem C
 Kim J-H, Jin S-A, Shim J-H, Cho YW. Reversible hydrogen storage in calcium
borohydride Ca(BH4)2. Scripta Mater 2008;58:481-3.
 Kim Y, Reed D, Lee Y-S, Lee JY, Shim J-H, Book D, et al. Identification of the
dehydrogenated product of Ca(BH4)2. J Phys Chem C 2009;113:5865-71.
 Kim Y, Reed D, Lee Y-S, Shim J-H, Han HN, Book D, et al. Hydrogenation reaction of
CaH2–CaB6–Mg mixture. J Alloy Compd 2010;492:597-600.
 Yartys VA, Denys RV, Webb CJ, Mæhlen JP, Gray EM, Blach T, et al. High pressure in
situ diffraction studies of metal–hydrogen systems. J Alloy Compd 2011;509, Supplement
 Oelerich W, Klassen T, Bormann R. Metal oxides as catalysts for improved hydrogen
sorption in nanocrystalline Mg-based materials. J Alloy Compd 2001;315:237-42.
 Barkhordarian G, Klassen T, Bormann R. Fast hydrogen sorption kinetics of
nanocrystalline Mg using Nb2O5 as catalyst. Scripta Mater 2003;49:213-7.
 Barkhordarian G, Klassen T, Bormann R. Patent pending. 2004.
 Dornheim M, Doppiu S, Barkhordarian G, Boesenberg U, Klassen T, Gutfleisch O, et al.
Hydrogen storage in magnesium-based hydrides and hydride composites. Scripta Mater
 Chupas PJ, Ciraolo MF, Hanson JC, Grey CP. In situ X-ray diffraction and solid-state
NMR study of the fluorination of γ-Al2O3 with HCF2Cl. J Am Chem Soc 2001;123:1694702.
 Chupas PJ, Chapman KW, Kurtz C, Hanson JC, Lee PL, Grey CP. A versatile sampleenvironment cell for non-ambient X-ray scattering experiments. J Appl Crystallogr
 http://www.photonic.saint-gobain.com/sapphire-tubes-rods.aspx access date: 10/2010.
 Friedrichs O, Aguey-Zinsou F, Fernández JRA, Sánchez-López JC, Justo A, Klassen T,
et al. MgH2 with Nb2O5 as additive, for hydrogen storage: Chemical, structural and kinetic
behavior with heating. Acta Mater 2006;54:105-10.